#------------------------------------------------------------------------------
#$Date: 2016-03-23 20:55:54 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179431 $
#$URL: svn://www.crystallography.net/cod/cif/4/33/28/4332875.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided the Crystal Eye server at
# http://wwmm.ch.cam.ac.uk/crystaleye/, created by Nick Day at the
# Peter Murray-Rust laboratory.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_4332875
loop_
_publ_author_name
'Sun, Junliang'
'Yang, Min'
'Li, Guobao'
'Yang, Tao'
'Liao, Fuhui'
'Wang, Yingxia'
'Xiong, Ming'
'Lin, Jianhua'
_publ_section_title
;
 New Barium Cobaltite Series Ban+1ConO3n+3(Co8O8):  Intergrowth
 Structure Containing Perovskite and CdI2-Type Layers
;
_journal_issue                   23
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              9151
_journal_page_last               9153
_journal_paper_doi               10.1021/ic060992v
_journal_volume                  45
_journal_year                    2006
_chemical_formula_sum            'Ba2 Co9 O14'
_chemical_formula_weight         1029.03
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            3
_cell_length_a                   5.6958(4)
_cell_length_b                   5.6958(4)
_cell_length_c                   28.909(4)
_cell_measurement_temperature    296(2)
_cell_volume                     812.22(14)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.942
_diffrn_measured_fraction_theta_max 0.942
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0362
_diffrn_reflns_av_sigmaI/netI    0.0308
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       38
_diffrn_reflns_limit_l_min       -43
_diffrn_reflns_number            2387
_diffrn_reflns_theta_full        33.29
_diffrn_reflns_theta_max         33.29
_diffrn_reflns_theta_min         2.11
_exptl_absorpt_coefficient_mu    20.627
_exptl_absorpt_correction_T_max  0.361
_exptl_absorpt_correction_T_min  0.150
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(SADABS; Bruker, 2001)'
_exptl_crystal_density_diffrn    6.312
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1401
_exptl_crystal_size_max          0.1
_exptl_crystal_size_mid          0.1
_exptl_crystal_size_min          0.05
_refine_diff_density_max         1.122
_refine_diff_density_min         -1.901
_refine_diff_density_rms         0.341
_refine_ls_extinction_coef       0.00093(12)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.005
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     34
_refine_ls_number_reflns         420
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.005
_refine_ls_R_factor_all          0.0266
_refine_ls_R_factor_gt           0.0258
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0168P)²+21.4689P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0565
_refine_ls_wR_factor_ref         0.0568
_reflns_number_gt                409
_reflns_number_total             420
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic060992vsup1.cif
_cod_data_source_block           r-3m
_cod_original_cell_volume        812.21(15)
_cod_original_sg_symbol_H-M      R-3m:H
_cod_database_code               4332875
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'y, x, -z'
'x-y, -y, -z'
'-x, -x+y, -z'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'y+2/3, x+1/3, -z+1/3'
'x-y+2/3, -y+1/3, -z+1/3'
'-x+2/3, -x+y+1/3, -z+1/3'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'y+1/3, x+2/3, -z+2/3'
'x-y+1/3, -y+2/3, -z+2/3'
'-x+1/3, -x+y+2/3, -z+2/3'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-y, -x, z'
'-x+y, y, z'
'x, x-y, z'
'-x+2/3, -y+1/3, -z+1/3'
'y+2/3, -x+y+1/3, -z+1/3'
'x-y+2/3, x+1/3, -z+1/3'
'-y+2/3, -x+1/3, z+1/3'
'-x+y+2/3, y+1/3, z+1/3'
'x+2/3, x-y+1/3, z+1/3'
'-x+1/3, -y+2/3, -z+2/3'
'y+1/3, -x+y+2/3, -z+2/3'
'x-y+1/3, x+2/3, -z+2/3'
'-y+1/3, -x+2/3, z+2/3'
'-x+y+1/3, y+2/3, z+2/3'
'x+1/3, x-y+2/3, z+2/3'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ba1 Ba 1.0000 1.0000 0.117118(15) 0.00938(15) Uani 1 6 d S
Co1 Co 1.0000 1.0000 0.0000 0.0053(2) Uani 1 12 d S
Co2 Co 1.5000 1.0000 0.0000 0.00401(17) Uani 1 4 d S
Co3 Co 1.3333 0.6667 0.1667 0.0043(2) Uani 1 12 d S
Co4 Co 1.3333 0.6667 0.07980(3) 0.0042(2) Uani 1 6 d S
Co5 Co 0.6667 1.3333 0.09989(3) 0.0063(2) Uani 1 6 d S
O1 O 1.1792(3) 0.8208(3) 0.03761(9) 0.0045(5) Uani 1 2 d S
O2 O 1.6667 1.3333 0.03371(17) 0.0049(8) Uani 1 6 d S
O3 O 1.0337(6) 1.5168(3) 0.12248(9) 0.0068(5) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 Ba1 O3 170.88(13) 2_875 2_765
O3 Ba1 O3 119.709(11) 2_875 3_575
O3 Ba1 O3 53.24(13) 2_765 3_575
O3 Ba1 O3 119.709(11) 2_875 1_545
O3 Ba1 O3 66.57(13) 2_765 1_545
O3 Ba1 O3 119.709(11) 3_575 1_545
O3 Ba1 O3 53.24(13) 2_875 .
O3 Ba1 O3 119.709(11) 2_765 .
O3 Ba1 O3 66.57(13) 3_575 .
O3 Ba1 O3 170.88(13) 1_545 .
O3 Ba1 O3 66.57(13) 2_875 3_675
O3 Ba1 O3 119.709(11) 2_765 3_675
O3 Ba1 O3 170.88(13) 3_575 3_675
O3 Ba1 O3 53.24(13) 1_545 3_675
O3 Ba1 O3 119.709(11) . 3_675
O3 Ba1 O1 123.48(7) 2_875 3_675
O3 Ba1 O1 59.92(8) 2_765 3_675
O3 Ba1 O1 59.92(7) 3_575 3_675
O3 Ba1 O1 94.50(6) 1_545 3_675
O3 Ba1 O1 94.50(6) . 3_675
O3 Ba1 O1 123.48(7) 3_675 3_675
O3 Ba1 O1 94.50(6) 2_875 .
O3 Ba1 O1 94.50(6) 2_765 .
O3 Ba1 O1 123.48(7) 3_575 .
O3 Ba1 O1 59.92(7) 1_545 .
O3 Ba1 O1 123.48(7) . .
O3 Ba1 O1 59.92(7) 3_675 .
O1 Ba1 O1 63.75(9) 3_675 .
O3 Ba1 O1 59.92(8) 2_875 2_765
O3 Ba1 O1 123.48(7) 2_765 2_765
O3 Ba1 O1 94.50(6) 3_575 2_765
O3 Ba1 O1 123.48(7) 1_545 2_765
O3 Ba1 O1 59.92(7) . 2_765
O3 Ba1 O1 94.50(6) 3_675 2_765
O1 Ba1 O1 63.75(9) 3_675 2_765
O1 Ba1 O1 63.75(9) . 2_765
O3 Ba1 O3 89.27(6) 2_875 26_455
O3 Ba1 O3 89.27(6) 2_765 26_455
O3 Ba1 O3 114.73(4) 3_575 26_455
O3 Ba1 O3 57.26(10) 1_545 26_455
O3 Ba1 O3 114.73(4) . 26_455
O3 Ba1 O3 57.26(10) 3_675 26_455
O1 Ba1 O3 145.94(4) 3_675 26_455
O1 Ba1 O3 108.68(8) . 26_455
O1 Ba1 O3 145.93(4) 2_765 26_455
O3 Ba1 O3 57.26(10) 2_875 27_655
O3 Ba1 O3 114.73(4) 2_765 27_655
O3 Ba1 O3 89.27(6) 3_575 27_655
O3 Ba1 O3 114.73(4) 1_545 27_655
O3 Ba1 O3 57.26(10) . 27_655
O3 Ba1 O3 89.27(6) 3_675 27_655
O1 Ba1 O3 145.93(4) 3_675 27_655
O1 Ba1 O3 145.94(4) . 27_655
O1 Ba1 O3 108.68(8) 2_765 27_655
O3 Ba1 O3 57.51(9) 26_455 27_655
O3 Ba1 O3 114.73(4) 2_875 25_675
O3 Ba1 O3 57.26(10) 2_765 25_675
O3 Ba1 O3 57.26(10) 3_575 25_675
O3 Ba1 O3 89.27(6) 1_545 25_675
O3 Ba1 O3 89.27(6) . 25_675
O3 Ba1 O3 114.73(4) 3_675 25_675
O1 Ba1 O3 108.68(9) 3_675 25_675
O1 Ba1 O3 145.94(4) . 25_675
O1 Ba1 O3 145.93(4) 2_765 25_675
O3 Ba1 O3 57.51(9) 26_455 25_675
O3 Ba1 O3 57.51(9) 27_655 25_675
O1 Co1 O1 180.00(12) 20_565 2_765
O1 Co1 O1 95.07(10) 20_565 21_655
O1 Co1 O1 84.93(10) 2_765 21_655
O1 Co1 O1 84.93(10) 20_565 .
O1 Co1 O1 95.07(10) 2_765 .
O1 Co1 O1 84.93(10) 21_655 .
O1 Co1 O1 84.93(10) 20_565 3_675
O1 Co1 O1 95.07(10) 2_765 3_675
O1 Co1 O1 180.00(12) 21_655 3_675
O1 Co1 O1 95.07(10) . 3_675
O1 Co1 O1 95.07(10) 20_565 19_775
O1 Co1 O1 84.93(10) 2_765 19_775
O1 Co1 O1 95.07(10) 21_655 19_775
O1 Co1 O1 180.00(12) . 19_775
O1 Co1 O1 84.93(10) 3_675 19_775
O1 Co1 Co2 137.54(5) 20_565 3_785
O1 Co1 Co2 42.46(5) 2_765 3_785
O1 Co1 Co2 42.46(5) 21_655 3_785
O1 Co1 Co2 90.0 . 3_785
O1 Co1 Co2 137.54(5) 3_675 3_785
O1 Co1 Co2 90.0 19_775 3_785
O1 Co1 Co2 42.46(5) 20_565 3_675
O1 Co1 Co2 137.54(5) 2_765 3_675
O1 Co1 Co2 137.54(5) 21_655 3_675
O1 Co1 Co2 90.0 . 3_675
O1 Co1 Co2 42.46(5) 3_675 3_675
O1 Co1 Co2 90.0 19_775 3_675
Co2 Co1 Co2 180.0 3_785 3_675
O1 Co1 Co2 90.0 20_565 1_455
O1 Co1 Co2 90.0 2_765 1_455
O1 Co1 Co2 137.54(5) 21_655 1_455
O1 Co1 Co2 137.54(5) . 1_455
O1 Co1 Co2 42.46(5) 3_675 1_455
O1 Co1 Co2 42.46(5) 19_775 1_455
Co2 Co1 Co2 120.0 3_785 1_455
Co2 Co1 Co2 60.0 3_675 1_455
O1 Co1 Co2 137.54(5) 20_565 2_765
O1 Co1 Co2 42.46(5) 2_765 2_765
O1 Co1 Co2 90.0 21_655 2_765
O1 Co1 Co2 137.54(5) . 2_765
O1 Co1 Co2 90.0 3_675 2_765
O1 Co1 Co2 42.46(5) 19_775 2_765
Co2 Co1 Co2 60.0 3_785 2_765
Co2 Co1 Co2 120.0 3_675 2_765
Co2 Co1 Co2 60.0 1_455 2_765
O1 Co1 Co2 42.46(5) 20_565 2_755
O1 Co1 Co2 137.54(5) 2_765 2_755
O1 Co1 Co2 90.0 21_655 2_755
O1 Co1 Co2 42.46(5) . 2_755
O1 Co1 Co2 90.0 3_675 2_755
O1 Co1 Co2 137.54(5) 19_775 2_755
Co2 Co1 Co2 120.0 3_785 2_755
Co2 Co1 Co2 60.0 3_675 2_755
Co2 Co1 Co2 120.0 1_455 2_755
Co2 Co1 Co2 180.0 2_765 2_755
O1 Co1 Co2 90.0 20_565 .
O1 Co1 Co2 90.0 2_765 .
O1 Co1 Co2 42.46(5) 21_655 .
O1 Co1 Co2 42.46(5) . .
O1 Co1 Co2 137.54(5) 3_675 .
O1 Co1 Co2 137.54(5) 19_775 .
Co2 Co1 Co2 60.0 3_785 .
Co2 Co1 Co2 120.0 3_675 .
Co2 Co1 Co2 180.0 1_455 .
Co2 Co1 Co2 120.0 2_765 .
Co2 Co1 Co2 60.0 2_755 .
O2 Co2 O2 180.0(2) 19_875 .
O2 Co2 O1 96.16(11) 19_875 21_655
O2 Co2 O1 83.84(11) . 21_655
O2 Co2 O1 83.84(11) 19_875 3_775
O2 Co2 O1 96.16(11) . 3_775
O1 Co2 O1 180.00(13) 21_655 3_775
O2 Co2 O1 83.84(11) 19_875 .
O2 Co2 O1 96.16(11) . .
O1 Co2 O1 93.58(17) 21_655 .
O1 Co2 O1 86.42(17) 3_775 .
O2 Co2 O1 96.16(11) 19_875 19_875
O2 Co2 O1 83.84(11) . 19_875
O1 Co2 O1 86.42(17) 21_655 19_875
O1 Co2 O1 93.58(17) 3_775 19_875
O1 Co2 O1 180.00(17) . 19_875
O2 Co2 Co4 85.17(12) 19_875 .
O2 Co2 Co4 94.83(12) . .
O1 Co2 Co4 136.67(9) 21_655 .
O1 Co2 Co4 43.33(9) 3_775 .
O1 Co2 Co4 43.33(9) . .
O1 Co2 Co4 136.67(9) 19_875 .
O2 Co2 Co4 94.83(12) 19_875 19_875
O2 Co2 Co4 85.17(12) . 19_875
O1 Co2 Co4 43.33(9) 21_655 19_875
O1 Co2 Co4 136.67(9) 3_775 19_875
O1 Co2 Co4 136.67(9) . 19_875
O1 Co2 Co4 43.33(9) 19_875 19_875
Co4 Co2 Co4 180.00(2) . 19_875
O2 Co2 Co2 138.16(8) 19_875 2_865
O2 Co2 Co2 41.84(8) . 2_865
O1 Co2 Co2 86.80(8) 21_655 2_865
O1 Co2 Co2 93.20(8) 3_775 2_865
O1 Co2 Co2 137.78(6) . 2_865
O1 Co2 Co2 42.22(6) 19_875 2_865
Co4 Co2 Co2 120.176(9) . 2_865
Co4 Co2 Co2 59.824(9) 19_875 2_865
O2 Co2 Co2 41.84(8) 19_875 2_755
O2 Co2 Co2 138.16(8) . 2_755
O1 Co2 Co2 93.20(8) 21_655 2_755
O1 Co2 Co2 86.80(8) 3_775 2_755
O1 Co2 Co2 42.22(6) . 2_755
O1 Co2 Co2 137.78(6) 19_875 2_755
Co4 Co2 Co2 59.824(9) . 2_755
Co4 Co2 Co2 120.176(9) 19_875 2_755
Co2 Co2 Co2 180.0 2_865 2_755
O2 Co2 Co1 90.0 19_875 .
O2 Co2 Co1 90.0 . .
O1 Co2 Co1 46.79(9) 21_655 .
O1 Co2 Co1 133.21(9) 3_775 .
O1 Co2 Co1 46.79(9) . .
O1 Co2 Co1 133.21(9) 19_875 .
Co4 Co2 Co1 90.0 . .
Co4 Co2 Co1 90.0 19_875 .
Co2 Co2 Co1 120.0 2_865 .
Co2 Co2 Co1 60.0 2_755 .
O2 Co2 Co2 41.84(8) 19_875 3_775
O2 Co2 Co2 138.16(8) . 3_775
O1 Co2 Co2 137.78(6) 21_655 3_775
O1 Co2 Co2 42.22(6) 3_775 3_775
O1 Co2 Co2 86.80(8) . 3_775
O1 Co2 Co2 93.20(8) 19_875 3_775
Co4 Co2 Co2 59.824(9) . 3_775
Co4 Co2 Co2 120.176(9) 19_875 3_775
Co2 Co2 Co2 120.0 2_865 3_775
Co2 Co2 Co2 60.0 2_755 3_775
Co1 Co2 Co2 120.0 . 3_775
O3 Co3 O3 81.87(12) 1_545 3_675
O3 Co3 O3 81.87(12) 1_545 2_865
O3 Co3 O3 81.87(12) 3_675 2_865
O3 Co3 O3 179.998(1) 1_545 25_775
O3 Co3 O3 98.13(13) 3_675 25_775
O3 Co3 O3 98.13(12) 2_865 25_775
O3 Co3 O3 98.13(13) 1_545 27_645
O3 Co3 O3 179.998(1) 3_675 27_645
O3 Co3 O3 98.13(12) 2_865 27_645
O3 Co3 O3 81.87(12) 25_775 27_645
O3 Co3 O3 98.13(12) 1_545 26_455
O3 Co3 O3 98.13(12) 3_675 26_455
O3 Co3 O3 180.0 2_865 26_455
O3 Co3 O3 81.87(12) 25_775 26_455
O3 Co3 O3 81.87(12) 27_645 26_455
O3 Co3 Co4 49.16(8) 1_545 .
O3 Co3 Co4 49.16(8) 3_675 .
O3 Co3 Co4 49.16(8) 2_865 .
O3 Co3 Co4 130.84(8) 25_775 .
O3 Co3 Co4 130.84(8) 27_645 .
O3 Co3 Co4 130.84(8) 26_455 .
O3 Co3 Co4 130.84(8) 1_545 25_765
O3 Co3 Co4 130.84(8) 3_675 25_765
O3 Co3 Co4 130.84(8) 2_865 25_765
O3 Co3 Co4 49.16(8) 25_775 25_765
O3 Co3 Co4 49.16(8) 27_645 25_765
O3 Co3 Co4 49.16(8) 26_455 25_765
Co4 Co3 Co4 180.0 . 25_765
O3 Co3 Ba1 52.559(4) 1_545 .
O3 Co3 Ba1 52.559(4) 3_675 .
O3 Co3 Ba1 115.63(8) 2_865 .
O3 Co3 Ba1 127.440(4) 25_775 .
O3 Co3 Ba1 127.440(4) 27_645 .
O3 Co3 Ba1 64.37(8) 26_455 .
Co4 Co3 Ba1 66.463(7) . .
Co4 Co3 Ba1 113.536(7) 25_765 .
O3 Co3 Ba1 52.559(4) 1_545 1_545
O3 Co3 Ba1 115.63(8) 3_675 1_545
O3 Co3 Ba1 52.559(4) 2_865 1_545
O3 Co3 Ba1 127.442(4) 25_775 1_545
O3 Co3 Ba1 64.37(8) 27_645 1_545
O3 Co3 Ba1 127.441(4) 26_455 1_545
Co4 Co3 Ba1 66.463(7) . 1_545
Co4 Co3 Ba1 113.537(7) 25_765 1_545
Ba1 Co3 Ba1 105.117(8) . 1_545
O3 Co3 Ba1 115.63(8) 1_545 1_655
O3 Co3 Ba1 52.559(4) 3_675 1_655
O3 Co3 Ba1 52.559(4) 2_865 1_655
O3 Co3 Ba1 64.37(8) 25_775 1_655
O3 Co3 Ba1 127.442(4) 27_645 1_655
O3 Co3 Ba1 127.441(4) 26_455 1_655
Co4 Co3 Ba1 66.463(7) . 1_655
Co4 Co3 Ba1 113.537(7) 25_765 1_655
Ba1 Co3 Ba1 105.117(8) . 1_655
Ba1 Co3 Ba1 105.117(8) 1_545 1_655
O3 Co3 Ba1 127.442(4) 1_545 25_765
O3 Co3 Ba1 127.442(4) 3_675 25_765
O3 Co3 Ba1 64.37(8) 2_865 25_765
O3 Co3 Ba1 52.559(4) 25_775 25_765
O3 Co3 Ba1 52.559(4) 27_645 25_765
O3 Co3 Ba1 115.62(8) 26_455 25_765
Co4 Co3 Ba1 113.538(7) . 25_765
Co4 Co3 Ba1 66.463(7) 25_765 25_765
Ba1 Co3 Ba1 180.0 . 25_765
Ba1 Co3 Ba1 74.883(8) 1_545 25_765
Ba1 Co3 Ba1 74.883(8) 1_655 25_765
O3 Co4 O3 83.34(14) 3_675 1_545
O3 Co4 O3 83.34(14) 3_675 2_865
O3 Co4 O3 83.34(14) 1_545 2_865
O3 Co4 O1 95.83(9) 3_675 .
O3 Co4 O1 95.83(9) 1_545 .
O3 Co4 O1 178.88(12) 2_865 .
O3 Co4 O1 178.88(12) 3_675 2_755
O3 Co4 O1 95.83(9) 1_545 2_755
O3 Co4 O1 95.83(9) 2_865 2_755
O1 Co4 O1 84.99(12) . 2_755
O3 Co4 O1 95.83(9) 3_675 3_775
O3 Co4 O1 178.88(12) 1_545 3_775
O3 Co4 O1 95.83(9) 2_865 3_775
O1 Co4 O1 84.99(12) . 3_775
O1 Co4 O1 84.99(12) 2_755 3_775
O3 Co4 Co3 50.15(9) 3_675 .
O3 Co4 Co3 50.15(9) 1_545 .
O3 Co4 Co3 50.15(9) 2_865 .
O1 Co4 Co3 128.74(8) . .
O1 Co4 Co3 128.74(8) 2_755 .
O1 Co4 Co3 128.73(8) 3_775 .
O3 Co4 Co2 138.13(6) 3_675 2_755
O3 Co4 Co2 94.37(9) 1_545 2_755
O3 Co4 Co2 138.13(6) 2_865 2_755
O1 Co4 Co2 42.62(6) . 2_755
O1 Co4 Co2 42.62(6) 2_755 2_755
O1 Co4 Co2 86.75(9) 3_775 2_755
Co3 Co4 Co2 144.519(11) . 2_755
O3 Co4 Co2 94.37(9) 3_675 .
O3 Co4 Co2 138.13(6) 1_545 .
O3 Co4 Co2 138.13(6) 2_865 .
O1 Co4 Co2 42.62(6) . .
O1 Co4 Co2 86.75(9) 2_755 .
O1 Co4 Co2 42.62(6) 3_775 .
Co3 Co4 Co2 144.519(11) . .
Co2 Co4 Co2 60.353(18) 2_755 .
O3 Co4 Co2 138.13(6) 3_675 3_775
O3 Co4 Co2 138.13(6) 1_545 3_775
O3 Co4 Co2 94.37(9) 2_865 3_775
O1 Co4 Co2 86.75(9) . 3_775
O1 Co4 Co2 42.62(6) 2_755 3_775
O1 Co4 Co2 42.62(6) 3_775 3_775
Co3 Co4 Co2 144.519(11) . 3_775
Co2 Co4 Co2 60.353(18) 2_755 3_775
Co2 Co4 Co2 60.353(18) . 3_775
O3 Co4 Ba1 55.633(11) 3_675 .
O3 Co4 Ba1 55.633(11) 1_545 .
O3 Co4 Ba1 121.98(10) 2_865 .
O1 Co4 Ba1 56.90(8) . .
O1 Co4 Ba1 124.448(12) 2_755 .
O1 Co4 Ba1 124.448(12) 3_775 .
Co3 Co4 Ba1 71.835(15) . .
Co2 Co4 Ba1 88.746(10) 2_755 .
Co2 Co4 Ba1 88.746(10) . .
Co2 Co4 Ba1 143.65(2) 3_775 .
O3 Co4 Ba1 55.633(11) 3_675 1_655
O3 Co4 Ba1 121.98(10) 1_545 1_655
O3 Co4 Ba1 55.633(11) 2_865 1_655
O1 Co4 Ba1 124.448(12) . 1_655
O1 Co4 Ba1 124.448(12) 2_755 1_655
O1 Co4 Ba1 56.90(8) 3_775 1_655
Co3 Co4 Ba1 71.835(15) . 1_655
Co2 Co4 Ba1 143.65(2) 2_755 1_655
Co2 Co4 Ba1 88.746(10) . 1_655
Co2 Co4 Ba1 88.746(10) 3_775 1_655
Ba1 Co4 Ba1 110.745(15) . 1_655
O2 Co5 O3 109.83(9) 1_455 .
O2 Co5 O3 109.83(9) 1_455 3_575
O3 Co5 O3 109.11(9) . 3_575
O2 Co5 O3 109.83(9) 1_455 2_775
O3 Co5 O3 109.11(9) . 2_775
O3 Co5 O3 109.11(9) 3_575 2_775
O2 Co5 Ba1 98.611(18) 1_455 .
O3 Co5 Ba1 58.96(7) . .
O3 Co5 Ba1 58.96(7) 3_575 .
O3 Co5 Ba1 151.56(9) 2_775 .
O2 Co5 Ba1 98.611(18) 1_455 1_565
O3 Co5 Ba1 58.96(7) . 1_565
O3 Co5 Ba1 151.56(9) 3_575 1_565
O3 Co5 Ba1 58.96(7) 2_775 1_565
Ba1 Co5 Ba1 117.799(9) . 1_565
O2 Co5 Ba1 98.611(18) 1_455 1_455
O3 Co5 Ba1 151.56(9) . 1_455
O3 Co5 Ba1 58.96(7) 3_575 1_455
O3 Co5 Ba1 58.96(7) 2_775 1_455
Ba1 Co5 Ba1 117.799(9) . 1_455
Ba1 Co5 Ba1 117.799(9) 1_565 1_455
O2 Co5 Ba1 180.0 1_455 25_675
O3 Co5 Ba1 70.17(9) . 25_675
O3 Co5 Ba1 70.17(9) 3_575 25_675
O3 Co5 Ba1 70.17(9) 2_775 25_675
Ba1 Co5 Ba1 81.390(18) . 25_675
Ba1 Co5 Ba1 81.389(18) 1_565 25_675
Ba1 Co5 Ba1 81.389(18) 1_455 25_675
Co2 O1 Co2 95.56(12) 2_755 .
Co2 O1 Co4 94.05(11) 2_755 .
Co2 O1 Co4 94.05(11) . .
Co2 O1 Co1 90.75(10) 2_755 .
Co2 O1 Co1 90.75(10) . .
Co4 O1 Co1 172.85(15) . .
Co2 O1 Ba1 132.03(6) 2_755 .
Co2 O1 Ba1 132.03(6) . .
Co4 O1 Ba1 88.84(9) . .
Co1 O1 Ba1 84.01(9) . .
Co2 O2 Co2 96.32(16) . 2_865
Co2 O2 Co2 96.32(16) . 3_785
Co2 O2 Co2 96.32(16) 2_865 3_785
Co2 O2 Co5 120.65(12) . 1_655
Co2 O2 Co5 120.65(12) 2_865 1_655
Co2 O2 Co5 120.65(12) 3_785 1_655
Co5 O3 Co4 120.32(15) . 1_565
Co5 O3 Co3 158.99(16) . 1_565
Co4 O3 Co3 80.69(12) 1_565 1_565
Co5 O3 Ba1 85.81(6) . 1_565
Co4 O3 Ba1 90.57(6) 1_565 1_565
Co3 O3 Ba1 94.56(6) 1_565 1_565
Co5 O3 Ba1 85.81(6) . .
Co4 O3 Ba1 90.57(6) 1_565 .
Co3 O3 Ba1 94.56(6) 1_565 .
Ba1 O3 Ba1 170.88(13) 1_565 .
Co5 O3 Ba1 76.09(9) . 25_675
Co4 O3 Ba1 163.60(15) 1_565 25_675
Co3 O3 Ba1 82.91(9) 1_565 25_675
Ba1 O3 Ba1 90.73(6) 1_565 25_675
Ba1 O3 Ba1 90.73(6) . 25_675
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ba1 O3 2.857(3) 2_875
Ba1 O3 2.857(3) 2_765
Ba1 O3 2.857(3) 3_575
Ba1 O3 2.857(3) 1_545
Ba1 O3 2.857(3) .
Ba1 O3 2.857(3) 3_675
Ba1 O1 2.900(3) 3_675
Ba1 O1 2.900(3) .
Ba1 O1 2.900(3) 2_765
Ba1 O3 3.259(3) 26_455
Ba1 O3 3.259(3) 27_655
Ba1 O3 3.259(3) 25_675
Co1 O1 2.076(3) 20_565
Co1 O1 2.076(3) 2_765
Co1 O1 2.076(3) 21_655
Co1 O1 2.076(3) .
Co1 O1 2.076(3) 3_675
Co1 O1 2.076(3) 19_775
Co1 Co2 2.8479(4) 3_785
Co1 Co2 2.8479(4) 3_675
Co1 Co2 2.8479(4) 1_455
Co1 Co2 2.8479(4) 2_765
Co1 Co2 2.8479(4) 2_755
Co1 Co2 2.8479(4) .
Co2 O2 1.911(2) 19_875
Co2 O2 1.911(2) .
Co2 O1 1.9228(18) 21_655
Co2 O1 1.9228(18) 3_775
Co2 O1 1.9228(18) .
Co2 O1 1.9228(18) 19_875
Co2 Co4 2.8328(8) .
Co2 Co4 2.8328(8) 19_875
Co2 Co2 2.8479(2) 2_865
Co2 Co2 2.8479(2) 2_755
Co2 Co2 2.8479(2) 3_775
Co3 O3 1.954(3) 1_545
Co3 O3 1.954(3) 3_675
Co3 O3 1.954(3) 2_865
Co3 O3 1.954(3) 25_775
Co3 O3 1.954(3) 27_645
Co3 O3 1.954(3) 26_455
Co3 Co4 2.5113(10) .
Co3 Co4 2.5114(10) 25_765
Co3 Ba1 3.5869(3) 1_545
Co3 Ba1 3.5869(3) 1_655
Co3 Ba1 3.5869(3) 25_765
Co4 O3 1.925(3) 3_675
Co4 O3 1.925(3) 1_545
Co4 O3 1.925(3) 2_865
Co4 O1 1.949(3) .
Co4 O1 1.949(3) 2_755
Co4 O1 1.949(3) 3_775
Co4 Co2 2.8328(8) 2_755
Co4 Co2 2.8328(8) 3_775
Co4 Ba1 3.4610(4) 1_655
Co5 O2 1.913(5) 1_455
Co5 O3 1.925(3) .
Co5 O3 1.925(3) 3_575
Co5 O3 1.925(3) 2_775
Co5 Ba1 3.3260(3) 1_565
Co5 Ba1 3.3260(3) 1_455
Co5 Ba1 3.3628(11) 25_675
O1 Co2 1.9228(18) 2_755
O2 Co2 1.911(2) 2_865
O2 Co2 1.911(2) 3_785
O2 Co5 1.913(5) 1_655
O3 Co4 1.925(3) 1_565
O3 Co3 1.954(3) 1_565
O3 Ba1 2.857(3) 1_565
O3 Ba1 3.259(3) 25_675
